stimuli-responsive microgels for the loading and release ... stimuli-responsive microgels for the...
Post on 17-Jun-2020
Embed Size (px)
at SciVerse ScienceDirect
Polymer 53 (2012) 5209e5231
Contents lists available
journal homepage: www.elsevier .com/locate/polymer
Stimuli-responsive microgels for the loading and release of functional compounds: Fundamental concepts and applications
Daniel Klinger, Katharina Landfester*
Max Planck Institute for Polymer Research, Ackermannweg 10, 55128 Mainz, Germany
a r t i c l e i n f o
Article history: Received 6 July 2012 Received in revised form 17 August 2012 Accepted 21 August 2012 Available online 1 September 2012
Keywords: Stimuli-responsive microgels Polymeric nanoparticles Polymeric networks Crosslinking Drug delivery
* Corresponding author. E-mail address: firstname.lastname@example.org (K
0032-3861� 2012 Elsevier Ltd. http://dx.doi.org/10.1016/j.polymer.2012.08.053
Open access under CC BY
a b s t r a c t
Stimuli-responsive microgels represent a highly interesting and unique class of materials since they exhibit exceptional properties which stem from the particular combination of their colloidal nature with their internal network structure. While this fascinating characteristic feature has been exploited in various different research fields and applications, the essential commonality for the successful devel- opment of all those diverse materials is a precise design of the respective microgels to adjust their functionality to a specific application. Regarding the delivery of functional compounds in particular, one of the main tasks is to combine an efficient loading process with a well defined release profile. A basic requirement to achieve this goal is a profound understanding of the underlying concepts of these material’s features and the impact of these basic models on the design and preparation of such highly functional materials exhibiting tailor-made properties. Therefore, in this review we present some of the important fundamental examinations on the influence of (tunable) network characteristics on loading and release profiles, basic synthetic concepts to realize these concepts and highlight several examples of different approaches to stimuli-responsive microgels for loading and release applications. By this, we wish to give the reader a broad overview of the design criteria and practical methodologies to control the functionality of microgels in order to encourage further development of highly interesting concepts and materials in this area of materials science.
� 2012 Elsevier Ltd. Open access under CC BY-NC-ND license.
Life itself is certainly the most sophisticated example for the utilization of selectively tailored polymers, polymer assemblies and interfaces to provide a specific chemical function and structure. Regarding natural biopolymers such as proteins, carbohydrates, and nucleic acids, the distinct position and nature of functional groups therein not only is the driving force to a particular three- dimensional structure and the resultant function of these mate- rials but also determines their response to external stimuli. Since these inherent features are the basis to construct and keep the complicated cell machinery running, understanding the funda- mental concept means learning a lesson from the most influential expert in property control by molecular design: nature [1,2].
Even though there is still a lot to learn anddiscover, early insights gained in thisfieldalreadyenabled the transferof several conceptsof biology to theworld of synthetic polymer chemistry . Concerning stimuli-sensitive macromolecular materials, the gathered
knowledge on the response mechanisms of biopolymers opened up new perspectives to mimic this behavior in synthetic systems. Moreover, it enabled the extension of this approach to the devel- opment of novel functional polymers exhibiting specific property changes triggered by signals non-existent in biologically-relevant areas [1,2]. While these stimuli can generally be realized either as changes in the materials environment (variations in pH, tempera- ture, or the presence/absence of chemical and biological compounds) or the application of an external field (light, electrical- or magnetic fields), the underlying similarities of all thesematerials are the triggered conformational and chemical changes of the respective polymeric system. The resulting fact that small signals are able to induce a comparably huge response apparent at the macro- scopic level renders these materials a fascinating research area.
Since the discovery of microgels as an intriguing class of such polymeric nanoscale materials, particularly the incorporation of stimuli-responsive properties into gel nanoparticles has gained increasing attention. In particular, regarding their utilization in loading and release applications, microgels, in comparison to other polymeric structures, exhibit exceptional properties. These stem from the unique combination of their colloidal nature (e.g. colloidal stability, high surface area, facile synthesis and control over particle
Delta:1_given name Delta:1_given name Delta:1_surname Delta:1_given name mailto:email@example.com www.sciencedirect.com/science/journal/00323861 http://www.elsevier.com/locate/polymer http://dx.doi.org/10.1016/j.polymer.2012.08.053 http://dx.doi.org/10.1016/j.polymer.2012.08.053 http://dx.doi.org/10.1016/j.polymer.2012.08.053 http://creativecommons.org/licenses/by-nc-nd/3.0/ http://creativecommons.org/licenses/by-nc-nd/3.0/
D. Klinger, K. Landfester / Polymer 53 (2012) 5209e52315210
size) with the inherent features of macroscopic hydrogels, i.e. their internal network structure (e.g. structural integrity in combination with fluid-like transport characteristics). Since the latter is charac- terized by such parameters as mesh size, polymer volume fraction, or the interactionwith embedded functional compounds, the ability to control these factors by the application of external triggers represents the underlying concept to stimuli-responsive microgels.
Here, we want to highlight some of the important fundamental examinations on the influence of (tunable) network characteristics on loading and release profiles as well as basic synthetic approaches to realize these concepts. These general considerations (obtained from fundamental research in this field) have shown that a specific stimuli-sensitive profile is the result of highly cooperative interactions and can be realized by precisely regulating not only the type but also the localization of a vast number of functional groups in a polymeric system. Since microgels for a specific loading and release application call for such a well defined stimuli-responsive behavior precisely adjusted to the respective requirements and settings, it can be stated that the key point to the successful development of such materials is to understand the importance of transferring fundamental insights in structure- and composition- property relationships to the design of specific synthetic pathways.
On the basis of these considerations, it becomes obvious that the development of novel and highly sophisticated artificial materials in this area is a result of a combination of specific foundations, concepts, and tools from diverse disciplines. In particular, the synergy between organic synthesis, polymer chemistry, colloidal science, highly accurate physical characterization methods as well as not only inorganic chemistry and nanotechnology but also the biomedical field, led to a multitude of stimuli-responsive microgels for a broad variety of applications such as catalysis, optics, sensors, and drug delivery [3e6].
Therefore, the aim of this review is to give the reader (especially from research fields different than the classic colloidal science) a broad overview of the design criteria and practical methodologies to control the functionality of microgels in order to encourage the further development of highly interesting concepts and materials in this area of materials science.
2. Polymeric gels: from macro to micro
Gelation of polymers was first investigated in 1931 by Carothers who polymerized multifunctional monomers by polycondensation. He suggested that this phenomenon is a result of linking polymer molecules into a three-dimensional network of infinitely large size . Since the polymer network consists of inter- and intramolec- ularly connected polymer chains, the entire gel network can indeed be considered as one macroscopic molecule whose size is theo- retically only limited by the dimensions of the containing vessel .
Starting from these early investigations, the development of new polymerization techniques and the understanding and resulting utilization of specific molecular interactions dramatically expanded the field of polymeric gels over the years. Hence, three- dimensional networks are no longer only formed by poly- condensation reactions in the presence of multifunctional branching units, but nowadays one can choose from a vast variety of different methods and concepts for the preparation of polymeric gels. These, in general, consist of (organic) polymer components which are crosslinked by either covalent or physical connecting points. Moreover, an additional prerequisite for gels is the ability of such networks to swell upon absorbing specific (solvent) mole- cules, thereby distinguishing them from other crosslinked poly- meric materials such as resins, elastomers or thermoset polymers.
Depending on the absorbed media, gels can be further classified into lyogels and aerogels. While the latter represent lightweight
highly porous materials, the unique combination of the structural integrity of a solid with